# Determination of Potassium, Sodium, and Total Alkalies in Portland Cement, Fly Ash, Admixtures, and Water of Concrete by a Simple Flow Injection Flame Photometric System

Authors: Jaroon Junsomboon; Jaroon Jakmunee
Journal: Journal of Automated Methods and Management in Chemistry
 (2011)

---

## Abstract

A simple flow injection with flame photometric detection has been developed for determination of sodium, potassium, and total alkalies in portland cement, fly ash, admixtures, and water of concrete. A liquid sample or a digest of solid sample was injected into a water carrier stream which flowed to a flame photometer. A change in emission intensity at a selected wavelength was recorded as a peak. An amplifier circuit was fabricated, which helped improve sensitivity of the flame photometer. Calibration graphs in the range of 0.05–1.0 mgL−1 and 1.0–20.0 mg L−1 were obtained with a detection limit of 0.02 mg L−1, for both potassium and sodium determination.  Relative standard deviations for 11 replicates of injecting of 10 mg L−1 potassium and sodium solutions were 1.69 and 1.79%, respectively. Sample throughput of 120 h−1 was achieved. The proposed method was successfully applied to portland cement, fly ash, admixtures, and water samples validated by the ASTM standard method and certified reference materials of portland cement.


---

## Body

## 1. Introduction

Concrete is the most widely used construction material in the world. It is composed of cement and other cementitious materials such as fly ash and slag cement, aggregates    (e.g., gravels, crushed rock, and sand), water, and chemical admixture [1]. Cement acts as binding material. It is mixed with water to produce cement paste that glues the aggregates together. Concrete has a good compressive strength (ca. 200 Kg cm−2), as the aggregates efficiently carry the compressive load. However, it is weak in its resistance to tension. Reinforced concrete is made by adding steel bars, steel fibers, glass fibers, or plastic fibers to concrete, in order to improve its tensile strength. Admixtures are materials that are added to give certain characteristics not obtainable with plain concrete mixes. They may help speed up or slow down the hydration of concrete and improve durability of concrete and plasticity or workability of fresh concrete. Since many reactions occur in concrete, some reactions are not desirable, especially the alkali-silica reaction (ASR). ASR is the neutralization reaction between alkaline cement paste and reactive noncrystalline (amorphous) silica, which is found in many common aggregates. This reaction produces swelling gel products which exerts an expansive pressure inside concrete. ASR occurs over time in concrete and can cause serious expansion and cracking of concrete, leading to critical structural problems. ASR can be mitigated by three complementary approaches; that is, limit the alkali metal contents of the cement, limiting the reactive silica content of the aggregate, and neutralizing the excessive alkalinity of cement at the early stage of the cement setting by adding very fine siliceous materials or pozzolanic materials to concrete mixture. Sodium hydroxide and potassium hydroxide are the most reactive alkalies in cement. Many standards set limits on the alkali as “equivalent sodium oxide (Na2O)” content of cement and other materials [2–4]. Equivalent sodium oxide is calculated as follows: (Na2O)e = Na2O + 0.658 K2O). Thus, it is important to determine sodium and potassium in cement and other materials for quality control of the products.Atomic absorption spectrophotometry (AAS) and flame emission spectrophotometry (FES), or flame photometry have been approved to be standard methods for determination of sodium and potassium in cement and materials for making concrete [2, 3]. Flow injection analysis (FIA) has been incorporated to these detectors in order to gain various advantages such as fast and convenient operation, on-line sample preparation, and high degrees of automation [5–18]. FAAS and FES are widely used as detection systems because they provide high sensitivity and selectivity. Other detection techniques which involve smaller instruments such as ion-selective electrode [19, 20] and turbidimetry [21] with FIA, also developed, but their selectivities are rather limited.In this work, we develop a simple FIA with FES detection for determination of sodium and potassium in materials of concrete. FIA improved performance of FES in terms of increasing sample throughput, helping to keep nubelizer and burner clean, and providing higher degrees of automation. A home-made amplification circuit was also incorporated to the FI-FES system in order to improve sensitivity and detection limit of the FES. The developed system was successfully applied for the analysis of cement, aggregates, and admixtures of concrete, so it would be suitable to be used as the automated analytical system for routine quality control of these materials.


## 2. Experimental

### 2.1. Chemicals

Analytical reagent grade chemicals were used and deionized water (obtained from a system of Milli-Q, Millipore, Sweden) was used throughout for preparation of solutions. A sodium standard stock solution (1000 mg L−1) was prepared by dissolving 0.2542 g of sodium chloride (Merck, Darmstadt, Germany) in 0.1 M hydrochloric acid and making up to a volume of 100 mL in a volumetric flask. A potassium standard stock solution (1000 mg L−1) was prepared by dissolving 0.1907 g of potassium chloride (Merck, Darmstadt, Germany) in 0.1 M hydrochloric acid and adjusting to the final volume of 100 mL. Working standard solutions of sodium and potassium were prepared daily by appropriately diluting their stock solutions with water. A 0.1 M hydrochloric acid solution was prepared by diluting concentrated hydrochloric acid (Merck, Darmstadt, Germany) with water.


### 2.2. Instrumentation and Procedure

The FI system used is depicted in Figure1. It is a simple single line FI setup consisting of a peristaltic pump (Ismatec, Switzerland), a six-port injection valve (Upchurch, USA), a flame emission spectrophotometer (Corning 410, Corning, Halstead, England), a home-made amplification/data acquisition unit, and a personal computer.Figure 1
FI manifold of flow injection flame photometric system for determination of Na and K; C = DI water carrier, S = standard/sample, P = peristaltic pump, I = injection valve, MC = mixing coil, W = waste, D = flame photometric detector, Amp/DAQ = data acquisition unit with amplifier (see Figure2), PC = personal computer.Figure2 illustrates a schematic diagram of the data acquisition unit with an amplifier circuit. Analog signal from the FES instrument was passed to the operational amplifier (Op amp) input. The signal was amplified by the Op amp which was connected as a noninverting amplifier circuit. Amplification gain could be set by adjusting selector switch (SW) to select a suitable amplification resistor (R2). Amplification gain is defined as 1 + R2/R1. The amplified signal was then passed to an analog to digital converter circuit (ADC) consisting of a 12 bit ADC integrated circuit, LTC1298, in order to convert the analog signal to digital signal which was suitable for recording by a computer. The data acquisition was performed by a Basic Stamp 2SX microcontroller, employing a software program written in-house in Visual Basic 6.0. The recorded data was imported to eDAQ chart software (eDAQ, Australia) for further evaluation for peak heights of the FIA peaks.Figure 2
Schematic diagram of an amplification and data acquisition unit. Resistor R1 = 2 K, R2 = 0–1000 K, amplification gain = 1 + R2/R1.Using the FI system as shown in Figure1, standard or sample solution was injected into a carrier stream and flowed to the FES burner. Output signal from the FES was amplified and continuously recorded on a personal computer as FIA peak. Peak height obtained was directly proportional to concentration of the analyte and could be used for construction of a calibration graph for determination of sodium or potassium in sample.


### 2.3. Sample Preparation

Cement and fly ash samples were prepared according to the standard method, ASTM C114-09 [2]. The sample was accurately weighed to 1.0000 g and put into a 150 mL beaker. Then 20 mL of water and 5 mL of concentrated hydrochloric acid were consecutively added, followed by adding water to the mark of 50 mL. The suspension was digested on a hot plate for about 15 min and the solution was filtered through a Whatman No. 40 filter paper into a 100 mL volumetric flask. Finally, water was added to the mark to obtain a solution ready for analysis.Sample of liquid admixture of concrete was prepared by using the standard method, BS EN 480-12: 1998 [3]. Briefly, sample was weighed accurately to 1.0000 g, put in a 150 mL beaker, added to 20 mL of water and 1 mL of (1 : 1) concentrated nitric acid. The solution was adjusted to 100 mL with water in a volumetric flask.Sample of water for making concrete (ground water and tab water) was prepared according to the standard method, AWWA: 1998 [22]. The sample was filtered through a Whatman No. 42 filter paper, and then 50 mL of sample was pipetted into a 150 mL beaker, added to 5 mL of conc. nitric acid, and digested on a hot plate to nearly dryness. The digested solution was filtered through a Whatman No. 42 filter paper into a 100 mL volumetric flask and adjusted to the mark with water.


## 2.1. Chemicals

Analytical reagent grade chemicals were used and deionized water (obtained from a system of Milli-Q, Millipore, Sweden) was used throughout for preparation of solutions. A sodium standard stock solution (1000 mg L−1) was prepared by dissolving 0.2542 g of sodium chloride (Merck, Darmstadt, Germany) in 0.1 M hydrochloric acid and making up to a volume of 100 mL in a volumetric flask. A potassium standard stock solution (1000 mg L−1) was prepared by dissolving 0.1907 g of potassium chloride (Merck, Darmstadt, Germany) in 0.1 M hydrochloric acid and adjusting to the final volume of 100 mL. Working standard solutions of sodium and potassium were prepared daily by appropriately diluting their stock solutions with water. A 0.1 M hydrochloric acid solution was prepared by diluting concentrated hydrochloric acid (Merck, Darmstadt, Germany) with water.


## 2.2. Instrumentation and Procedure

The FI system used is depicted in Figure1. It is a simple single line FI setup consisting of a peristaltic pump (Ismatec, Switzerland), a six-port injection valve (Upchurch, USA), a flame emission spectrophotometer (Corning 410, Corning, Halstead, England), a home-made amplification/data acquisition unit, and a personal computer.Figure 1
FI manifold of flow injection flame photometric system for determination of Na and K; C = DI water carrier, S = standard/sample, P = peristaltic pump, I = injection valve, MC = mixing coil, W = waste, D = flame photometric detector, Amp/DAQ = data acquisition unit with amplifier (see Figure2), PC = personal computer.Figure2 illustrates a schematic diagram of the data acquisition unit with an amplifier circuit. Analog signal from the FES instrument was passed to the operational amplifier (Op amp) input. The signal was amplified by the Op amp which was connected as a noninverting amplifier circuit. Amplification gain could be set by adjusting selector switch (SW) to select a suitable amplification resistor (R2). Amplification gain is defined as 1 + R2/R1. The amplified signal was then passed to an analog to digital converter circuit (ADC) consisting of a 12 bit ADC integrated circuit, LTC1298, in order to convert the analog signal to digital signal which was suitable for recording by a computer. The data acquisition was performed by a Basic Stamp 2SX microcontroller, employing a software program written in-house in Visual Basic 6.0. The recorded data was imported to eDAQ chart software (eDAQ, Australia) for further evaluation for peak heights of the FIA peaks.Figure 2
Schematic diagram of an amplification and data acquisition unit. Resistor R1 = 2 K, R2 = 0–1000 K, amplification gain = 1 + R2/R1.Using the FI system as shown in Figure1, standard or sample solution was injected into a carrier stream and flowed to the FES burner. Output signal from the FES was amplified and continuously recorded on a personal computer as FIA peak. Peak height obtained was directly proportional to concentration of the analyte and could be used for construction of a calibration graph for determination of sodium or potassium in sample.


## 2.3. Sample Preparation

Cement and fly ash samples were prepared according to the standard method, ASTM C114-09 [2]. The sample was accurately weighed to 1.0000 g and put into a 150 mL beaker. Then 20 mL of water and 5 mL of concentrated hydrochloric acid were consecutively added, followed by adding water to the mark of 50 mL. The suspension was digested on a hot plate for about 15 min and the solution was filtered through a Whatman No. 40 filter paper into a 100 mL volumetric flask. Finally, water was added to the mark to obtain a solution ready for analysis.Sample of liquid admixture of concrete was prepared by using the standard method, BS EN 480-12: 1998 [3]. Briefly, sample was weighed accurately to 1.0000 g, put in a 150 mL beaker, added to 20 mL of water and 1 mL of (1 : 1) concentrated nitric acid. The solution was adjusted to 100 mL with water in a volumetric flask.Sample of water for making concrete (ground water and tab water) was prepared according to the standard method, AWWA: 1998 [22]. The sample was filtered through a Whatman No. 42 filter paper, and then 50 mL of sample was pipetted into a 150 mL beaker, added to 5 mL of conc. nitric acid, and digested on a hot plate to nearly dryness. The digested solution was filtered through a Whatman No. 42 filter paper into a 100 mL volumetric flask and adjusted to the mark with water.


## 3. Results and Discussion

### 3.1. Optimization of the FI-FES for Determination of Sodium

FI-FES system as shown in Figure1 was used with the preliminary conditions as follows: flow rate of the carrier stream of 2.0 mL min−1, sample volume of 200 μL, and no mixing coil connected between an injection valve and a detector. An amplifier gain was optimized for determination of sodium in concentration range of 1–20 mg L−1 which is the normal analytical range used in routine analysis. The amplifier gain of 30× was selected as it gave an analog signal of the 20 mg L−1 Na close to 5 V which is the maximum allowable input signal of the ADC circuit.Effect of flow rate of the carrier stream was investigated by injecting a series of sodium standard solution (1–20 mg L−1) into the system and a calibration graph was constructed by plotting peak height obtained versus sodium concentration for each flow rate used. Calibration equations, y=0.181x-0.037, r2=0.9994, y=0.181x+0.095, r2=0.9975 and   y=0.218x+0.078, r2=0.9955 were obtained for flow rate of 1.0, 2.0, and 3.0 mL min−1, respectively. Flow rate of 3.0 mL min−1 was chosen since it provided adequate sensitivity and high sample throughput (120 h−1). Flow rate of higher than 3.0 mL min−1 was not investigated in order to avoid high consumption of the carrier.Effect of mixing coil length was then studied in the range of 0–100 cm. Calibration equations,y=0.217x+0.078, r2=0.9956, y=0.182x+0.056, r2=0.9993, y=0.155x+0.014, r2=0.9998 and y=0.133x+0.025, r2=0.9996 were obtained for mixing coil lengths of 0, 25, 50, and 100 cm, respectively. The longer the coil length the smaller the slope and observed due to the higher dispersion of the injected solution, so the system without mixing coil was selected for further experiments.Effect of sample volume in the range of 75–200μL was investigated. It was found that the higher the sample volume the higher sensitivity was obtained, that is, calibration equations, y=0.142x+0.037, r2=0.9988, y=0.177x+0.044, r2=0.9992 and y=0.218x+0.077, r2=0.9955 for sample volumes of 75, 100, and 200 μL, respectively, were obtained. Sample volume of 100 μL was chosen as it provided enough sensitivity for the analysis of sample.


### 3.2. Optimization of FI-FES for Determination of Potassium

Employing FI-FES system as shown in Figure1 and the following preliminary conditions: carrier flow rate of 2.0 mL min−1, sample volume of 200 μL, and no mixing coil, an amplifier gain was optimized for the determination of potassium in the concentration range of 1–20 mg L−1. The amplifier gain of 50× was selected as it gave an analog signal of 20 mg L−1 K close to 5 V which is the maximum allowable input signal of the ADC circuit.Effect of flow rate of carrier stream was studied similar to Section3.1. Calibration equations for the injection of potassium standard solutions in the range of 1–20 mg L−1 with carrier flow rates of 1.0, 2.0, and 3.0 mL min−1 were y=0.215x-0.032, r2=0.9991, y=0.238x-0.001, r2=0.9994 and y=0.244x+0.113, r2=0.9892, respectively. Flow rate of 2.0 mL min−1 was chosen because it provided good sensitivity and linearity.The studied mixing coil lengths of 0, 25, 50, and 100 cm provided calibration equations ofy=0.220x-0.051, r2=0.9987, y=0.196x-0.067, r2=0.9990 and y=0.178x-0.051, r2=0.9976, respectively. The FI system without mixing coil was selected for further studies since it gave high sensitivity.Effect of sample volume was investigated. Calibration equations ofy=0.185x-0.067, r2=0.9984, y=0.222x-0.053, r2=0.9996 and y=0.2378x-0.001, r2=0.9994 were obtained for sample volumes of 75, 100, and 200 μL, respectively. Sample volume of 100 μL was selected as it provided higher sensitivity and narrower peak.By adding lithium into a carrier solution to reduce ionization of sodium and potassium, the sensitivity could be slightly enhanced as shown in Figure3. However, at 2.0% (w/v) Li the fluctuation of baseline was observed. Thus, water carrier without ionization-suppression buffer was chosen since it used no chemical and helped to keep the nebulizer and burner of FES instrument clean.Figure 3
Effect of Li added to carrier solution on sensitivity of sodium and potassium determination by FI-FES.


### 3.3. Analytical Characteristics

Under the selected conditions, flow rate of water carrier of 3.0 mL min−1, sample volume of 100 μL, and no mixing coil, two linear calibration ranges for determination of sodium were attained, that is, y=0.284x+0.004, r2=0.9970 for 0.05–1.0 mg L−1 Na (with amplifier gain 50×) and y=0.181x+0.001, r2=0.9989 for 1.0–20.0 mg L−1 Na (with amplifier gain 30×). FIA grams of the standard solutions of sodium and some samples are depicted in Figure 4.Figure 4
FIA grams of sodium standard solutions and some samples. From left to right standard solution 1.0, 3.0, 5.0, 8.0, 10.0, 15.0, and 20.0 mg L−1 Na and sample’s number 1–20, triplicate injections for each solution.Two linear calibration graphs were also obtained for the determination of potassium, that is,y=1.931x+0.1138, r2=0.9966 for 0.05–1.0 mg L−1 K (with amplifier gain 500×) and y=0.218x-0.134, r2=0.9996 for 1.0–20.0 mg L−1 K (with amplifier gain 50×). Figure 5 illustrates FIA grams of potassium standard solutions and some samples.Figure 5
FIA grams of potassium standard solutions and some samples. From left to right standard solution 1.0, 3.0, 5.0, 8.0, 10.0, 15.0, and 20.0 mg L−1 K and sample’s number 1–20, triplicate injections for each solution.Detection limits (3 times the standard deviation of the blank/slope of analytical curve) of 0.02 mg L−1 were achieved for both sodium and potassium determinations. Relative standard deviations for 11 replicates of injection of 10 mg L−1 of sodium and potassium were 1.79 and 1.69, respectively. Sample throughput of 120 h−1 was obtained.


### 3.4. Validation of the Method

Recovery study was performed by spiking standard solution of sodium or potassium into the prepared solutions of cement, fly ash, and concrete admixture solutions. Recoveries were obtained in the ranges of 89–102% and 86–106% for sodium and potassium, respectively (Table1).Table 1
Recoveries of sodium and potassium determined by FI-FES.
SampleNa concentration found (mg L−1)K concentration found (mg L−1)Original sampleWith 5 mg L−1 Na added% RecoveryOriginal sampleWith 5 mg L−1 K added% RecoveryCement9.76±0.0414.35±0.0191.812.37±0.2516.66±0.0985.8Fly ash4.32±0.058.80±0.0289.64.98±0.079.31±0.1786.6Admixture 18.77±0.0113.86±0.18101.80.00±0.005.31±0.08106.2Admixture 26.19±0.1110.65±0.0589.21.87±0.186.59±0.1594.4Certified reference materials of portland cements were analyzed by the proposed method. The results are summarized in Table2. The contents of Na2O and K2O as determined by the proposed FI-FES method were in acceptable range of the certified values, indicating that the method could be applied for these samples.Table 2
Analyses of certified reference materials of portland cement by FI-FES.
Sample% Na2O% K2OFI-FESCertified valueFI-FESCertified valueCRM 18890.134±0.0010.110.264±0.0020.32CRM 6330.661±0.0020.640.149±0.0030.16CRM 6380.151±0.0010.120.572±0.0020.59


### 3.5. Application to Real Samples

The developed method was applied to cement, fly ash, admixture solutions, and water for making concrete. The samples were prepared as described in Section  2.3 before injecting the obtained solution into the FI system. Thirty-five samples were analyzed, and the contents of sodium and potassium, reported as % Na2O and % K2O are summarized in Table 3.Table 3
Contents of sodium, potassium, and total alkalies determined by FI-FES and batchwise FES methods.
Sample% Na2O% K2O% Total alkaliesFI-FESFESFI-FESFESFI-FESFESCement10.124±0.0010.121±0.0010.299±0.0020.292±0.0010.3210.31320.267±0.0020.262±0.0010.332±0.0040.322±0.0020.4850.47430.122±0.0010.117±0.0010.268±0.0020.265±0.0010.2990.29140.052±0.0010.047±0.0010.053±0.0010.045±0.0010.0870.07650.437±0.0020.435±0.0020.600±0.0070.637±0.0030.8310.85560.076±0.0010.070±0.0010.131±0.0020.128±0.0010.1620.15570.108±0.0010.107±0.0010.277±0.0020.273±0.0010.2910.28680.139±0.0010.134±0.0010.294±0.0040.290±0.0010.3330.32590.098±0.0020.091±0.0010.249±0.0030.247±0.0010.2620.254100.118±0.0010.113±0.0010.326±0.0050.326±0.0010.3330.327Fly ash110.079±0.0020.074±0.0010.039±0.0010.035±0.0010.1040.098120.026±0.0010.023±0.0010.035±0.0010.033±0.0010.0490.045131.608±0.0351.595±0.0081.339±0.0161.455±0.0072.4892.553140.547±0.0060.574±0.0130.571±0.0130.627±0.0010.9220.986150.155±0.0040.147±0.0010.172±0.0020.167±0.0010.2680.257161.664±0.0371.658±0.0081.407±0.0121.552±0.0072.5902.680171.989±0.0161.983±0.0081.543±0.0171.664±0.0073.0053.077180.098±0.0010.093±0.0010.177±0.0030.174±0.0010.2140.207191.771±0.0341.763±0.0081.490±0.0051.639±0.0072.7512.841201.839±0.0231.837±0.0151.333±0.0061.461±0.0122.7152.798Admixture210.159±0.0010.162±0.0010.014±0.0010.012±0.0010.1680.171220.158±0.0030.159±0.0010.008±0.0010.005±0.0010.1640.162230.153±0.0050.150±0.0030.020±0.0010.017±0.0010.1660.161244.584±0.0994.555±0.0140.014±0.0010.011±0.0014.5934.562252.182±0.0262.165±0.0080.186±0.0010.199±0.0012.3052.296260.157±0.0050.153±0.0030.017±0.0010.015±0.0010.1680.163270.195±0.0010.186±0.0010.016±0.0010.013±0.0010.2060.195280.161±0.0010.157±0.0010.012±0.0010.010±0.0010.1690.164290.170±0.0060.167±0.0010.009±0.0010.005±0.0010.1750.170300.178±0.0050.168±0.0010.022±0.0010.022±0.0010.1920.183Water310.203±0.0040.197±0.0010.043±0.0010.043±0.0010.2320.225320.196±0.0040.194±0.0010.043±0.0010.043±0.0010.2240.223330.190±0.0010.186±0.0010.044±0.0010.045±0.0010.2190.216340.235±0.0050.234±0.0010.048±0.0010.050±0.0010.2670.267350.239±0.0050.227±0.0010.051±0.0020.053±0.0010.2720.261The routinely used batchwise FES method [2–4] was also employed for analyses of all samples for comparison. It was found that the results obtained from both methods were not significantly different, as evaluated by t-test at 95% confidence level [23], tcalc.=0.022 versus ttable=2.000 for sodium and  tcalc.=0.166 versus ttable=2.000 for potassium. Correlation plots of the results from both methods gave linear equations, y=0.995x-0.177, r2=0.9999 for sodium and y=1.097x-1.032, r2=0.9994 for potassium, respectively. However, the developed FI-FES method was faster and more convenient to perform than the standard method. Analytical signal was recorded and could be retrieved for further evaluation at a later time.Total alkali contents reported as equivalent sodium oxide are also summarized in Table3. It was found that total alkali contents found in most samples of cement, admixture, and water were lower than the permissible value of the Thai Industrial Standard which is set to be not higher than 0.6% [4]. Several samples of fly ash contained total alkalies at level higher than the permissible value.


### 3.6. Comparison to Other Methods

Analytical features of the developed method were compared to some reported methods as shown in Table4. The proposed FI-FES system has high sensitivity and provides low limit of detection. It has comparable precision and sample throughput to most of the reported methods. This work is the first report on the application of FI-FES for determination of potassium, sodium, and total alkalies in cement and other materials for making concrete.Table 4
Analytical features of the developed FI-FES method versus some reported methods.
Method*DeterminationPrincipleSampleLinear rangeLOD (mg L−1)R.S.D. (%)H−1Ref.MSFI-FESKIn-line dilution of sample and FESSoil, table wine1–2000 mg L−1—0.8–3.414[3]FI-FES, FI- FAASNa, K, Mg, CaFIA combination with FES and FAASGround water, domestic water——1.7–2.7128[6]FI-FAASMn, Pb, Zn, Ca, Mg, Fe,Onlinedilution device of sample with FAASCements0.05–0.25% w/v———[7]FI-FAASNa, K, Ca, Mg,Direct FI-FAASFruits0.1–1.0 mg L−1 Na1.5–6.0 mg L−1 K—1.0-2.060[8]FI-FAASAl, Fe, Ca, Mg, Na, KOnline dilution in a stirred chamber with FAASCeramic materials0.2–14 mg L−1 Na0.2–10 mg L−1 K0.240.730.752.1248[9]FI-FAASFe, Ca, Mg, Na, KUsing a variation volume injector with FAAS and FESCeramic materials2–8 mg L−1 Na2–10 mg L−1 K0.10.050.80.560[10]FI-FESLi, Na, KSplitting system with FESBlood serum14–140 mmol L−1 Na0.5–5.0 mmol L−1 K——108[11]FI-FES, FI- FAASNa, K, Ca, MgFES and FAAS  with on-line dilutionBeer10–130 mg L−1 Na100–500 mg L−1 K—1.6–3.8120–200[12]FI-FESNa, KUsing two dialysis units with FESVegetables206.4–2896 mg L−1 K81.02–1158 mg L−1 Na—<1.6, <1.7120–150[13]FI-FESKUsing needle valve connected to nitrogen cylinder and the Buchner flask with FESGasoline,  lubricating oils4–16 mg kg−12–15 mg kg−1—3.040–100[14]FI-FES, FI-UV-VisNa, K, Cl−Analysis of three components with online dialysis in series with FES and UV/VisBlood serum110–160 mM Na2–7 mM K—0.7–1.0106[15]FI-AAS, FI- FESCa, Mg, KDirect FI-FAAS and FI-FESPlant material——0.5–1.0300[16]FI-FESLi, Na, K, CaUsing gradient scanning standard addition with FESSoil, water20–80 mg L−1—2.5–4.6—[17]MSFI-FESKMSFIA system and inline microwave digestion with FESPlant20–200 mg g−10.48 mg g−12.5–4.028[18]FI-FESNa, K, total AlkaliesFI-FES with amplifier circuit used for improvement of sensitivityPortland cement, fly ash, admixture and water of concrete0.05–1.0 mg L−11.0–20.0 mg L−10.021.7–1.8120This work*FI = flow injection, MSFI = multisyringe flow injection, FES = flame emission spectrometry, FAAS = flame atomic absorption spectrometry.


## 3.1. Optimization of the FI-FES for Determination of Sodium

FI-FES system as shown in Figure1 was used with the preliminary conditions as follows: flow rate of the carrier stream of 2.0 mL min−1, sample volume of 200 μL, and no mixing coil connected between an injection valve and a detector. An amplifier gain was optimized for determination of sodium in concentration range of 1–20 mg L−1 which is the normal analytical range used in routine analysis. The amplifier gain of 30× was selected as it gave an analog signal of the 20 mg L−1 Na close to 5 V which is the maximum allowable input signal of the ADC circuit.Effect of flow rate of the carrier stream was investigated by injecting a series of sodium standard solution (1–20 mg L−1) into the system and a calibration graph was constructed by plotting peak height obtained versus sodium concentration for each flow rate used. Calibration equations, y=0.181x-0.037, r2=0.9994, y=0.181x+0.095, r2=0.9975 and   y=0.218x+0.078, r2=0.9955 were obtained for flow rate of 1.0, 2.0, and 3.0 mL min−1, respectively. Flow rate of 3.0 mL min−1 was chosen since it provided adequate sensitivity and high sample throughput (120 h−1). Flow rate of higher than 3.0 mL min−1 was not investigated in order to avoid high consumption of the carrier.Effect of mixing coil length was then studied in the range of 0–100 cm. Calibration equations,y=0.217x+0.078, r2=0.9956, y=0.182x+0.056, r2=0.9993, y=0.155x+0.014, r2=0.9998 and y=0.133x+0.025, r2=0.9996 were obtained for mixing coil lengths of 0, 25, 50, and 100 cm, respectively. The longer the coil length the smaller the slope and observed due to the higher dispersion of the injected solution, so the system without mixing coil was selected for further experiments.Effect of sample volume in the range of 75–200μL was investigated. It was found that the higher the sample volume the higher sensitivity was obtained, that is, calibration equations, y=0.142x+0.037, r2=0.9988, y=0.177x+0.044, r2=0.9992 and y=0.218x+0.077, r2=0.9955 for sample volumes of 75, 100, and 200 μL, respectively, were obtained. Sample volume of 100 μL was chosen as it provided enough sensitivity for the analysis of sample.


## 3.2. Optimization of FI-FES for Determination of Potassium

Employing FI-FES system as shown in Figure1 and the following preliminary conditions: carrier flow rate of 2.0 mL min−1, sample volume of 200 μL, and no mixing coil, an amplifier gain was optimized for the determination of potassium in the concentration range of 1–20 mg L−1. The amplifier gain of 50× was selected as it gave an analog signal of 20 mg L−1 K close to 5 V which is the maximum allowable input signal of the ADC circuit.Effect of flow rate of carrier stream was studied similar to Section3.1. Calibration equations for the injection of potassium standard solutions in the range of 1–20 mg L−1 with carrier flow rates of 1.0, 2.0, and 3.0 mL min−1 were y=0.215x-0.032, r2=0.9991, y=0.238x-0.001, r2=0.9994 and y=0.244x+0.113, r2=0.9892, respectively. Flow rate of 2.0 mL min−1 was chosen because it provided good sensitivity and linearity.The studied mixing coil lengths of 0, 25, 50, and 100 cm provided calibration equations ofy=0.220x-0.051, r2=0.9987, y=0.196x-0.067, r2=0.9990 and y=0.178x-0.051, r2=0.9976, respectively. The FI system without mixing coil was selected for further studies since it gave high sensitivity.Effect of sample volume was investigated. Calibration equations ofy=0.185x-0.067, r2=0.9984, y=0.222x-0.053, r2=0.9996 and y=0.2378x-0.001, r2=0.9994 were obtained for sample volumes of 75, 100, and 200 μL, respectively. Sample volume of 100 μL was selected as it provided higher sensitivity and narrower peak.By adding lithium into a carrier solution to reduce ionization of sodium and potassium, the sensitivity could be slightly enhanced as shown in Figure3. However, at 2.0% (w/v) Li the fluctuation of baseline was observed. Thus, water carrier without ionization-suppression buffer was chosen since it used no chemical and helped to keep the nebulizer and burner of FES instrument clean.Figure 3
Effect of Li added to carrier solution on sensitivity of sodium and potassium determination by FI-FES.


## 3.3. Analytical Characteristics

Under the selected conditions, flow rate of water carrier of 3.0 mL min−1, sample volume of 100 μL, and no mixing coil, two linear calibration ranges for determination of sodium were attained, that is, y=0.284x+0.004, r2=0.9970 for 0.05–1.0 mg L−1 Na (with amplifier gain 50×) and y=0.181x+0.001, r2=0.9989 for 1.0–20.0 mg L−1 Na (with amplifier gain 30×). FIA grams of the standard solutions of sodium and some samples are depicted in Figure 4.Figure 4
FIA grams of sodium standard solutions and some samples. From left to right standard solution 1.0, 3.0, 5.0, 8.0, 10.0, 15.0, and 20.0 mg L−1 Na and sample’s number 1–20, triplicate injections for each solution.Two linear calibration graphs were also obtained for the determination of potassium, that is,y=1.931x+0.1138, r2=0.9966 for 0.05–1.0 mg L−1 K (with amplifier gain 500×) and y=0.218x-0.134, r2=0.9996 for 1.0–20.0 mg L−1 K (with amplifier gain 50×). Figure 5 illustrates FIA grams of potassium standard solutions and some samples.Figure 5
FIA grams of potassium standard solutions and some samples. From left to right standard solution 1.0, 3.0, 5.0, 8.0, 10.0, 15.0, and 20.0 mg L−1 K and sample’s number 1–20, triplicate injections for each solution.Detection limits (3 times the standard deviation of the blank/slope of analytical curve) of 0.02 mg L−1 were achieved for both sodium and potassium determinations. Relative standard deviations for 11 replicates of injection of 10 mg L−1 of sodium and potassium were 1.79 and 1.69, respectively. Sample throughput of 120 h−1 was obtained.


## 3.4. Validation of the Method

Recovery study was performed by spiking standard solution of sodium or potassium into the prepared solutions of cement, fly ash, and concrete admixture solutions. Recoveries were obtained in the ranges of 89–102% and 86–106% for sodium and potassium, respectively (Table1).Table 1
Recoveries of sodium and potassium determined by FI-FES.
SampleNa concentration found (mg L−1)K concentration found (mg L−1)Original sampleWith 5 mg L−1 Na added% RecoveryOriginal sampleWith 5 mg L−1 K added% RecoveryCement9.76±0.0414.35±0.0191.812.37±0.2516.66±0.0985.8Fly ash4.32±0.058.80±0.0289.64.98±0.079.31±0.1786.6Admixture 18.77±0.0113.86±0.18101.80.00±0.005.31±0.08106.2Admixture 26.19±0.1110.65±0.0589.21.87±0.186.59±0.1594.4Certified reference materials of portland cements were analyzed by the proposed method. The results are summarized in Table2. The contents of Na2O and K2O as determined by the proposed FI-FES method were in acceptable range of the certified values, indicating that the method could be applied for these samples.Table 2
Analyses of certified reference materials of portland cement by FI-FES.
Sample% Na2O% K2OFI-FESCertified valueFI-FESCertified valueCRM 18890.134±0.0010.110.264±0.0020.32CRM 6330.661±0.0020.640.149±0.0030.16CRM 6380.151±0.0010.120.572±0.0020.59


## 3.5. Application to Real Samples

The developed method was applied to cement, fly ash, admixture solutions, and water for making concrete. The samples were prepared as described in Section  2.3 before injecting the obtained solution into the FI system. Thirty-five samples were analyzed, and the contents of sodium and potassium, reported as % Na2O and % K2O are summarized in Table 3.Table 3
Contents of sodium, potassium, and total alkalies determined by FI-FES and batchwise FES methods.
Sample% Na2O% K2O% Total alkaliesFI-FESFESFI-FESFESFI-FESFESCement10.124±0.0010.121±0.0010.299±0.0020.292±0.0010.3210.31320.267±0.0020.262±0.0010.332±0.0040.322±0.0020.4850.47430.122±0.0010.117±0.0010.268±0.0020.265±0.0010.2990.29140.052±0.0010.047±0.0010.053±0.0010.045±0.0010.0870.07650.437±0.0020.435±0.0020.600±0.0070.637±0.0030.8310.85560.076±0.0010.070±0.0010.131±0.0020.128±0.0010.1620.15570.108±0.0010.107±0.0010.277±0.0020.273±0.0010.2910.28680.139±0.0010.134±0.0010.294±0.0040.290±0.0010.3330.32590.098±0.0020.091±0.0010.249±0.0030.247±0.0010.2620.254100.118±0.0010.113±0.0010.326±0.0050.326±0.0010.3330.327Fly ash110.079±0.0020.074±0.0010.039±0.0010.035±0.0010.1040.098120.026±0.0010.023±0.0010.035±0.0010.033±0.0010.0490.045131.608±0.0351.595±0.0081.339±0.0161.455±0.0072.4892.553140.547±0.0060.574±0.0130.571±0.0130.627±0.0010.9220.986150.155±0.0040.147±0.0010.172±0.0020.167±0.0010.2680.257161.664±0.0371.658±0.0081.407±0.0121.552±0.0072.5902.680171.989±0.0161.983±0.0081.543±0.0171.664±0.0073.0053.077180.098±0.0010.093±0.0010.177±0.0030.174±0.0010.2140.207191.771±0.0341.763±0.0081.490±0.0051.639±0.0072.7512.841201.839±0.0231.837±0.0151.333±0.0061.461±0.0122.7152.798Admixture210.159±0.0010.162±0.0010.014±0.0010.012±0.0010.1680.171220.158±0.0030.159±0.0010.008±0.0010.005±0.0010.1640.162230.153±0.0050.150±0.0030.020±0.0010.017±0.0010.1660.161244.584±0.0994.555±0.0140.014±0.0010.011±0.0014.5934.562252.182±0.0262.165±0.0080.186±0.0010.199±0.0012.3052.296260.157±0.0050.153±0.0030.017±0.0010.015±0.0010.1680.163270.195±0.0010.186±0.0010.016±0.0010.013±0.0010.2060.195280.161±0.0010.157±0.0010.012±0.0010.010±0.0010.1690.164290.170±0.0060.167±0.0010.009±0.0010.005±0.0010.1750.170300.178±0.0050.168±0.0010.022±0.0010.022±0.0010.1920.183Water310.203±0.0040.197±0.0010.043±0.0010.043±0.0010.2320.225320.196±0.0040.194±0.0010.043±0.0010.043±0.0010.2240.223330.190±0.0010.186±0.0010.044±0.0010.045±0.0010.2190.216340.235±0.0050.234±0.0010.048±0.0010.050±0.0010.2670.267350.239±0.0050.227±0.0010.051±0.0020.053±0.0010.2720.261The routinely used batchwise FES method [2–4] was also employed for analyses of all samples for comparison. It was found that the results obtained from both methods were not significantly different, as evaluated by t-test at 95% confidence level [23], tcalc.=0.022 versus ttable=2.000 for sodium and  tcalc.=0.166 versus ttable=2.000 for potassium. Correlation plots of the results from both methods gave linear equations, y=0.995x-0.177, r2=0.9999 for sodium and y=1.097x-1.032, r2=0.9994 for potassium, respectively. However, the developed FI-FES method was faster and more convenient to perform than the standard method. Analytical signal was recorded and could be retrieved for further evaluation at a later time.Total alkali contents reported as equivalent sodium oxide are also summarized in Table3. It was found that total alkali contents found in most samples of cement, admixture, and water were lower than the permissible value of the Thai Industrial Standard which is set to be not higher than 0.6% [4]. Several samples of fly ash contained total alkalies at level higher than the permissible value.


## 3.6. Comparison to Other Methods

Analytical features of the developed method were compared to some reported methods as shown in Table4. The proposed FI-FES system has high sensitivity and provides low limit of detection. It has comparable precision and sample throughput to most of the reported methods. This work is the first report on the application of FI-FES for determination of potassium, sodium, and total alkalies in cement and other materials for making concrete.Table 4
Analytical features of the developed FI-FES method versus some reported methods.
Method*DeterminationPrincipleSampleLinear rangeLOD (mg L−1)R.S.D. (%)H−1Ref.MSFI-FESKIn-line dilution of sample and FESSoil, table wine1–2000 mg L−1—0.8–3.414[3]FI-FES, FI- FAASNa, K, Mg, CaFIA combination with FES and FAASGround water, domestic water——1.7–2.7128[6]FI-FAASMn, Pb, Zn, Ca, Mg, Fe,Onlinedilution device of sample with FAASCements0.05–0.25% w/v———[7]FI-FAASNa, K, Ca, Mg,Direct FI-FAASFruits0.1–1.0 mg L−1 Na1.5–6.0 mg L−1 K—1.0-2.060[8]FI-FAASAl, Fe, Ca, Mg, Na, KOnline dilution in a stirred chamber with FAASCeramic materials0.2–14 mg L−1 Na0.2–10 mg L−1 K0.240.730.752.1248[9]FI-FAASFe, Ca, Mg, Na, KUsing a variation volume injector with FAAS and FESCeramic materials2–8 mg L−1 Na2–10 mg L−1 K0.10.050.80.560[10]FI-FESLi, Na, KSplitting system with FESBlood serum14–140 mmol L−1 Na0.5–5.0 mmol L−1 K——108[11]FI-FES, FI- FAASNa, K, Ca, MgFES and FAAS  with on-line dilutionBeer10–130 mg L−1 Na100–500 mg L−1 K—1.6–3.8120–200[12]FI-FESNa, KUsing two dialysis units with FESVegetables206.4–2896 mg L−1 K81.02–1158 mg L−1 Na—<1.6, <1.7120–150[13]FI-FESKUsing needle valve connected to nitrogen cylinder and the Buchner flask with FESGasoline,  lubricating oils4–16 mg kg−12–15 mg kg−1—3.040–100[14]FI-FES, FI-UV-VisNa, K, Cl−Analysis of three components with online dialysis in series with FES and UV/VisBlood serum110–160 mM Na2–7 mM K—0.7–1.0106[15]FI-AAS, FI- FESCa, Mg, KDirect FI-FAAS and FI-FESPlant material——0.5–1.0300[16]FI-FESLi, Na, K, CaUsing gradient scanning standard addition with FESSoil, water20–80 mg L−1—2.5–4.6—[17]MSFI-FESKMSFIA system and inline microwave digestion with FESPlant20–200 mg g−10.48 mg g−12.5–4.028[18]FI-FESNa, K, total AlkaliesFI-FES with amplifier circuit used for improvement of sensitivityPortland cement, fly ash, admixture and water of concrete0.05–1.0 mg L−11.0–20.0 mg L−10.021.7–1.8120This work*FI = flow injection, MSFI = multisyringe flow injection, FES = flame emission spectrometry, FAAS = flame atomic absorption spectrometry.


## 4. Conclusion

FI-FES method was developed and successfully applied for determination of sodium and potassium in cement and materials of concrete. Amplifier circuit and data acquisition unit were incorporated to the system for improving sensitivity and continuous recording of signal from the FES instrument. FI acts as a sample introduction system for FES and also provides various advantages such as that it is fast and convenient analysis, the small volume of sample (100μL) used in FI helps improve the cleanliness of the nebulizer and burner of the FES, and the system has higher degrees of automation. With further incorporation of an autosampler, the system should be more appropriate for routine analysis.



---

*Source: 742656-2011-06-21.xml*